Characterization of a Synthetic Nano-Polycrystalline ... ... Synthetic nano-polycrystalline diamond
Embed Size (px)
Transcript of Characterization of a Synthetic Nano-Polycrystalline ... ... Synthetic nano-polycrystalline diamond
Synthetic nano-polycrystalline diamond (NPD)may be one of the most important developments in synthetic diamond production in recent years. This transparent brownish yellow material is pro- duced not by CVD or traditional HPHT synthesis methods, but rather in a multi-anvil press by a sin- tering process that converts high-purity graphite di- rectly into synthetic diamond. According to the developer of the process, the conversion time aver- ages 10–20 minutes (though can be less than 10 min- utes) at 15 gigapascals and 2,300–2,500°C (T. Irifune, pers. comm., 2012). These pressures and tempera- tures are far higher than those used in the HPHT syn-
thesis of single-crystal diamond. The material con- sists of randomly oriented nanoscale-sized synthetic diamond crystallites that have been bonded tightly together to form what may be thought of as an ultra- hard synthetic diamond ceramic.
A recent article by Skalwold (2012) documented a transparent 5 mm NPD sphere, and served as means to introduce this new synthetic diamond’s develop- ment and some of its properties. Soon after that arti- cle was published, Dr. Tetsuo Irifune, director of Ehime University’s Geodynamics Research Center (GRC), once again offered one of the authors (EAS) an exclusive opportunity to study this unique material. This time the specimen was a 0.88 ct faceted round brilliant (figure 1). In collaboration with researchers at GIA, an analysis of its gemological and spectro- scopic properties was undertaken to establish gem identification criteria. Further work on this material will be conducted by author EAS and by GIA as more samples become available.
A potential new synthetic gem material in the form of a faceted 0.88 ct brownish yellow nano- polycrystalline diamond (NPD) has undergone a full gemological examination, including detailed spectroscopic analysis, for the first time. While the material’s implications for the gem industry are still unknown, NPD’s optical characteristics along with manufacturing improvements make it a po- tentially important synthetic for gemologists to be aware of, even though very few samples have been faceted and future production costs and availability for gem purposes are uncertain. Fea- tures seen with magnification may provide an in- dication of its nano-polycrystalline nature, and the identification of this material can be con- firmed by spectroscopy and other advanced test- ing methods. NPD is an entirely new kind of synthetic diamond, and its development illustrates the ongoing research on diamond properties for a number of important applications beyond the field of gemology.
188 NOTES & NEW TECHNIQUES GEMS & GEMOLOGY FALL 2012
CHARACTERIZATION OF A SYNTHETIC NANO-POLYCRYSTALLINE DIAMOND GEMSTONE Elise A. Skalwold, Nathan Renfro, James E. Shigley, and Christopher M. Breeding
NOTES & NEW TECHNIQUES
See end of article for About the Authors and Acknowledgments. GEMS & GEMOLOGY, Vol. 48, No. 3, pp. 188–192, http://dx.doi.org/10.5741/GEMS.48.3.188. © 2012 Gemological Institute of America
Figure 1. This 0.88 ct synthetic nano-polycrystalline diamond, produced by direct conversion from graphite at high temperatures and pressures, repre- sents a completely new type of transparent gem mate- rial. Photo by Robert Weldon.
NEW Skalwold Notes & New Tech fall 2012_Layout 1 9/27/12 11:06 AM Page 188
As initially reported by Skalwold et al. (2012), while this transparent gem material shares some similarities with natural and synthetic single-crystal diamond, it also has properties that are sufficiently distinctive to be recognizable by gem-testing labora- tories. Given that there are only five known faceted samples in existence, the opportunity to characterize it with the assistance of a gemological laboratory was a singular opportunity.
PRODUCTION Relatively swift advancements have been made in the manufacturing process of NPD. In less than a decade since the successful production of this material was first reported (Irifune et al., 2003), improvements have resulted in relatively large pieces suitable for a number of applications, most notably for diamond anvils used in high-pressure research. For this purpose, two NPD cylinders are produced per week, generally measuring 6.5–9 mm in diameter and 6.5–8 mm in length (a maximum of 10 mm in each dimension is possible). But if the GRC’s Botchan multi-anvil press were to produce only NPD, up to 10 cylinders could be made each week. The pieces recovered from the press have a slight surface texture, caused by the tantalum cap-
sule in which the graphite-to-NPD conversion takes place (see figure 4 of Skalwold, 2012). These cylinders are cut by a combination of specialized lasers and pol- ishing techniques. The material requires nontradi- tional cutting and polishing methods because of its polycrystalline nature and polishing hardness. Unlike natural and other synthetic diamonds, NPD is uni- formly hard in all directions at the macro scale (al- though hardness varies on the nano scale).
Efforts are now under way at the GRC to produce colorless NPD. Marketing of the material is still in its infancy, and pricing for industrial use has yet to be established (T. Irifune, pers. comm., 2012).
MATERIALS AND METHODS A 0.88 ct round brilliant studied for this report meas- ured 6.13 × 6.10 × 3.78 mm. It was graded for color and clarity using standard GIA procedures. Basic gemolog- ical properties were collected (table 1), and additional testing was performed with a Presidium GEM Mini- DiamondMaster and a DTC DiamondSure screening device. The sample was examined with a Nikon SMZ- 1500 binocular gemological microscope under several lighting configurations. Deep-ultraviolet (~230 nm ex- citation) fluorescence images were captured using a DTC DiamondView instrument.
Visible absorption spectra were recorded with the sample cooled to liquid-nitrogen temperature (~77 K) using a custom-made Ocean Optics high-resolution spectrometer. Infrared absorption spectra were recorded with a Thermo-Nicolet Magna IR 760 spec- trometer, while Raman and photoluminescence (PL) spectra were measured with a Renishaw InVia Raman spectrometer. PL spectra were recorded at liquid-ni- trogen temperature using four excitation wavelengths (325, 488, 514, and 633 nm).
NOTES & NEW TECHNIQUES GEMS & GEMOLOGY FALL 2012 189
TABLE 1. Basic gemological properties of the NPD sample.
Fancy Deep brownish yellow
Slightly Included (SI1)
Slightly hazy or cloudy
Over the limits of the standard refractometer
Moderate chalky reddish orange
Weak reddish orange
Positive for diamond
Referred for further testing; not “passed” as natural diamond
Roiled appearance; one black and numerous pinpoint inclusions; patchy clouds of color zoning
In Brief • Synthetic nano-polycrystalline diamond (NPD) consists of nanoscale-sized synthetic diamond crystallites bonded together using an HPHT sintering process.
• A 0.88 ct brownish yellow round brilliant, one of five faceted NPD gems currently in existence, was charac- terized for this report.
• Key identifying properties include a hazy, roiled ap- pearance and distinctive mid-IR, visible-range, and photoluminescence spectra.
• This sample was cut from early production, and fu- ture NPD material may not show the same diagnostic features.
NEW Skalwold Notes & New Tech fall 2012_Layout 1 9/27/12 11:06 AM Page 189
RESULTS AND DISCUSSION The GIA color and clarity grades, as well as basic gemological properties, are shown in table 1. With magnification, we observed numerous whitish pin- point inclusions along with a single larger black in- clusion, patchy clouds of color zoning, and a roiled appearance (figure 2). This last feature was much like the effect sometimes seen in the hessonite variety of grossular, and it appeared to cause the sample’s slight haziness when viewed in the face-up position. The black inclusion showed a dominant broad Raman peak at 1078 cm–1, but we were unable to identify a mineral phase from the spectrum. Observation with crossed polarizing filters showed a cross-hatched or tatami-like strain pattern in several orientations, with no apparent variation in the color, intensity, or distri- bution of the pattern depending on direction (figure 3). While the hazy, roiled appearance is quite unusual, visual features alone should not be considered com- pletely diagnostic for NPD, but rather as indications that laboratory testing is needed.
Fluorescence imaging using the DiamondView showed orangy red luminescence with an irregular structure (figure 4). This unusual patchy appearance bears some resemblance to the networks or “webs” often seen in fluorescence images of natural type II di- amonds. The orangy red luminescence seems to arise from boundaries between what appear to be larger ag- gregates of the nano-crystallites. This distinctive lumi-
nescence is similar in appearance and color to that gen- erated by N-V optical centers in diamond.